General Route to Three-Dimensional Framework Uranyl Transition Metal Phosphates with Atypical Structural Motifs: The Case Examples of Cs2{(UO2)4[Co(H2O)2]2(HPO4)(PO4)4} and Cs3+x[(UO2)3CuH4-x(PO4)5]·H2O
Shvareva, Tatiana Y.; Albrecht-Schmitt, Thomas E.; Inorganic Chemistry 45 (2006) 1900–1902; doi:10.1021/ic051922b

data_4331939
_publ_section_title
;
 General Route to Three-Dimensional Framework Uranyl Transition Metal
 Phosphates with Atypical Structural Motifs:&#x00A0; The Case Examples of
 Cs2{(UO2)4[Co(H2O)2]2(HPO4)(PO4)4} and
 Cs3+x[(UO2)3CuH4-x(PO4)5]&#x00B7;H2O
;
_journal_issue                   5
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              1900
_journal_page_last               1902
_journal_paper_doi               10.1021/ic051922b
_journal_volume                  45
_journal_year                    2006
_chemical_formula_sum            'Co2 Cs2 O32 P5 U4'
_chemical_formula_weight         2002.65
_chemical_name_common            'cesium uranyl cobalt phosphate'
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           15
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 99.2420(10)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   18.0551(8)
_cell_length_b                   10.7478(5)
_cell_length_c                   15.3504(7)
_cell_measurement_reflns_used    all
_cell_measurement_temperature    193(2)
_cell_measurement_theta_max      28.28
_cell_measurement_theta_min      2.21
_cell_volume                     2940.1(2)
_computing_cell_refinement       SMART,SAINT
_computing_data_collection       SMART
_computing_data_reduction        SAINT
_computing_molecular_graphics    'SHELXP-97 (Sheldrick, 1997)'
_computing_publication_material  'SHELXCIF-97 (Sheldrick, 2000)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      193(2)
_diffrn_detector_area_resol_mean 0
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device_type  'Bruker APEX'
_diffrn_measurement_method       '0.3 wide w/exposures'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0421
_diffrn_reflns_av_sigmaI/netI    0.0326
_diffrn_reflns_limit_h_max       24
_diffrn_reflns_limit_h_min       -24
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_number            14656
_diffrn_reflns_theta_full        28.28
_diffrn_reflns_theta_max         28.28
_diffrn_reflns_theta_min         2.21
_diffrn_standards_decay_%        0
_diffrn_standards_interval_count na
_diffrn_standards_interval_time  na
_diffrn_standards_number         na
_exptl_absorpt_coefficient_mu    25.886
_exptl_absorpt_correction_T_max  0.3778
_exptl_absorpt_correction_T_min  0.1013
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   SHELXPREP
_exptl_crystal_colour            orange
_exptl_crystal_density_diffrn    4.524
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       plate
_exptl_crystal_F_000             3452
_exptl_crystal_size_max          0.16
_exptl_crystal_size_mid          0.16
_exptl_crystal_size_min          0.08
_refine_diff_density_max         4.074
_refine_diff_density_min         -1.200
_refine_diff_density_rms         0.290
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.047
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     209
_refine_ls_number_reflns         3629
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.047
_refine_ls_R_factor_all          0.0337
_refine_ls_R_factor_gt           0.0281
_refine_ls_shift/su_max          0.014
_refine_ls_shift/su_mean         0.001
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0339P)^2^+46.5648P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0677
_refine_ls_wR_factor_ref         0.0692
_reflns_number_gt                3220
_reflns_number_total             3629
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic051922bsup1.cif
_cod_data_source_block           c2c
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_crystal_density_meas' value 'not measured' was changed to '?'
- the value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 3008 2015-01-20 13:52:24Z robertas 
;
_cod_original_sg_symbol_H-M      C2/c
_cod_database_code               4331939